SSP421 Body Basics
Download SSP421 Body Basics...
Self-study Programme 421
What springs to mind when you think about a vehicle? Normally the drive, the engine, the performance and the image come first. But what would a car be without its body? It is the central component of a vehicle that connects all other vehicle components and, at the same time, manages to accommodate the passengers. It meets high technical requirements as well as the comfort expectations of passengers. Furthermore the body in particular bears the characteristic face of a vehicle and thus also of the car brand.
The self-study programme portrays the design and function of new developments. The contents will not be updated.
A modern body needs to retain a good condition, if possible, for the whole “life” of the car so that no unnecessary costs arise. This prevents a fast moral decline of a vehicle model and the brand will be held in high esteem. It is also important that damage to a body that occurs in any future accidents can be repaired and this highquality vehicle component can thus retain its properties and appearance. This self-study programme will explain the basic associations of material science, steel production and the treatment processes leading up to painting. It will lay the foundations for better understanding of the procedures should body repairs be necessary.
For current testing, adjustment and repair instructions, refer to the relevant service literature.
Contents Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Historical background . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4 Bodies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6 Basics - Materials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8 Basics - General information on materials . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8 Basics - Steel. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14 Basics - Treatment of steel. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 24 Basics - Aluminium . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 28 Steels for Body Construction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Classification of steels for body construction . . . . . . . . . . . . . . . . . . . . . . . . . . Increasing the strength of steel. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Body structure. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
30 30 31 38
Basics - Process Engineering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Manufacture of semi-finished products. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Tailored blanks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Joining processes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Coating processes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
40 40 46 48 56
Corrosion Protection . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Pre-treatment . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Seam sealing . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Stone chip protection. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Protection against galvanic corrosion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Painting . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
60 60 61 62 63 65
Repair . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 66 Basics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 66 Repair methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 67 Glossary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 74 The glossary provides explanations of the CAPITALISED terms
Introduction Historical background Introduction Car bodies yesterday and today - how have requirements and tasks of car bodies changed over the course of technical progress? To begin with, let us define the term “body”, which refers to the complete coachwork of a motor vehicle. Historically, the first superstructure on a vehicle with wheels could be considered as the start of body development. We should then also include the first open and later closed motor carriages. We will describe bodies in the context of motor vehicles throughout this self-study programme.
Non-load-bearing body The first bodies were not load-bearing, i.e. they were built on a frame or a chassis. Both ladder frames and tubular frames were used. Ladder frames are still used for lorries and off-road vehicles today. Bodies were not necessarily linked to one vehicle manufacturer. There were chassis manufacturers and coachbuilders. This allowed bodies to be adapted to and built onto different drivable chassis as required. Later on bodies were produced using a platform frame. The body structure was placed on a platform frame that had been specially designed for it and was then attached. Only then was it fitted onto the drivable chassis.
… from the start of motor vehicle production to this day …
Motor carriage Wood/steel
Separate body on drivable chassis, e.g. Ford Model T
Monocoque bodies Engineers looked for solutions to make bodies without a separate, heavy frame as it became necessary to reduce weight in car construction. The resulting body featured a structure that could support itself. This development was also aided by technical progress in sheet metal processing. In this design, the load-bearing body structures are joined together securely and permanently using different joining techniques, for example, welding, soldering and bonding. This method of construction is the general standard in car manufacturing today.
Use of materials The first bodies were made of wood, to which an outer coating of lacquer, fabric or plastic was added to improve the appearance and to also protect it from the elements. Modern bodies are increasingly not just optimised in terms of structure and cross-sections. Special tailor-made materials are being used more and more for specific body areas. The materials are distinguished by their respective composition and their treatment. These different materials are used to continually improve the ability of specific sections of the body to bear mechanical stress and resist corrosion. Above all, steel is used as a material. Aluminium and plastics are also being used more to create lightweight constructions.
S421_081 Body with platform frame
Current monocoque body
Introduction Bodies Bodies are frequently only perceived and understood as a design. People normally only consider the technical issues and comfort as an afterthought. In a nutshell, the body is first and foremost the part of a vehicle that allows passengers to be transported - it is the actual “transport case” for the people being carried.
Requirements for bodies
Structure of a body
As a result of technical progress, today’s bodies have an increasingly complex range of tasks to perform:
The body can be split into two main areas: ●
Transport space for passengers
Fulfilment of human needs, for example, comfort, noise insulation etc.
Due to safety requirements, the inner part of the body structure, also called the passenger cell, needs to be particularly resistant to deformation.
Accommodation of all technical components for drive and power transmission
Accommodation of all technical components for convenience systems
Accommodation of heating, ventilation and airconditioning systems
Accommodation of all safety systems
Design of the body for optimum protection against possible interior and exterior damage, e.g. in accidents
the inner body structure and the outer panels of the body structure
The front and rear ends of the body should allow optimum absorption and reduction of impact energy (crumple zones to meet safety requirements in a crash). This also applies increasingly for the side sections and the roofs of modern vehicles.
Repairs to a body Repairs to the inner body structure are very complex due to its sturdy configuration. Parts fastened to the body structure with bolts (body outer skin) are replaced if badly damaged.
The structure of a body will be shown using the bodies of the current Golf and Passat as examples. The body shows the internal body structure together with parts of the outer panels.
Body of Golf model year 2009
Body structure, outer panels transparent
With outer panels
Body of Passat model year 2006
Body structure, outer panels transparent
With outer panels
Basics - Materials Basics - General information on materials On modern bodies, specially configured materials are increasingly being used for specific body parts. In order to explain the reasons for the respective materials used, we will look at some principles of material science.
Crystalline structures All substances are made from different types of ATOMS (iron, sodium, gold, nitrogen, oxygen etc.) regardless of their state of matter (gas, liquid or solid). The ATOMS behave like solid balls, whose size varies depending on their nature. The following descriptions cover the relationships with the crystalline structures using metals as an example. When the metals are still in liquid state during melting, the ATOMS move randomly without staying in a set position.
When the materials become solid upon cooling, the ATOMS stop moving and arrange themselves in a set three-dimensional form, i.e. “crystalline structure”. The crystalline structure can be reduced to the respective smallest basic unit. In its simplest form, the basic unit can be, for example, simple cubic. Depending on the type of material, body-centred cubic and face-centred cubic or even hexagonal crystalline forms, for example, are possible in addition to the simple cubic forms. The crystalline structure type determines characteristic material properties like density, HARDNESS or melting point.
Basic unit (simple cubic)
The crystal lattice shown is a random section of a crystalline structure. The ATOMS highlighted in yellow in the illustration show an example of a basic unit of the crystalline structure - in this case a simple cubic crystal. The possible crystalline forms are explained in more detail on the next page.
Metals mostly crystallise in three crystalline forms: ●
Body-centred cubic crystal The METAL IONS arrange themselves so that the connecting lines between the ions form a cube. Another metal ion is located in the centre of the cube. This crystallisation type is found in chrome, molybdenum, vanadium and tungsten as well as in iron below approx. 900°C.
METAL IONS = electrically charged atoms
Face-centred cubic crystal The basic form of the crystal is also a cube. In addition to the eight METAL IONS at the corners, there is one ion in the centre of the six side surfaces. This crystallisation type is found, for example, in lead, aluminium, copper and nickel as well as in iron above approx. 900°C.
Hexagonal crystal The basic form of this crystal is a prism with hexagonal top and bottom surfaces. There is also a METAL ION in the centre of the top and bottom surfaces. In addition, three further METAL IONS are arranged inside the crystal. This crystallisation type is found, for example, in magnesium, titanium and zinc.
Basics - Materials Metal structure An arrangement only forms once solidification begins. Formation of crystallisation seeds begins at the points where the solidification temperature is reached first.
In liquid molten metal, METAL IONS and free ELECTRONS move randomly among each other. There is no specific arrangement.
Liquid molten metal
METAL IONS Continuing solidification
Start of solidification
Crystallisation seeds Complete solidification
Grain boundaries S421_089
As solidification continues, METAL IONS are deposited on these seeds and crystal lattices form. The crystal lattices continue to grow until they meet other neighbouring crystal lattices that are also growing. They cannot grow any further.
The crystals formed after complete solidification are irregular in their exterior form - they are also called crystallite or grains - they form the structure of a metal.
Iron is not used in its pure form for technical applications. Instead it is used in a wide range of ALLOYS. Iron and alloy components are melted together. The alloy additions dissolve in the iron base metal during this process. Different structure types are formed depending on the mixing ratio of iron and alloy components.
Structure types Solid solution alloy
Structure with substitutional solid solution crystals
When ATOMS from the base metal are replaced by an ion from the alloy metal in a crystal, this is known as a substitutional SOLID SOLUTION.
If the ions of the alloy metal arrange themselves between the METAL IONS, this is known as an interstitial SOLID SOLUTION .
Structure with interstitial solid solution crystals
Grain boundary S421_090
Multi-phase alloy Structure with multiple phases
If alloy components do not mix upon solidification of the melt and each component forms its own crystals, this is known as a multi-phase alloy.
Plain steel has one special feature. The alloy component in this case is carbon. It is chemically bonded in the steel as iron carbide (cementite) and forms thin layers between the grains of the iron crystals (ferrite) - these grains are called pearlite.
Structure of plain steel
Basics - Materials Mechanical properties The mechanical properties of materials are established in laboratory tests. Tensile testing for determining the strength of materials is the most common.
During the test, the load required to deform the sample until it breaks and the extent of deformation is determined. A stress-strain curve (load in relation to the original cross-section of the sample) can then be drawn up from the results.
In tensile testing, samples of the test material are subjected to a rising pulling force at room temperature. All samples must have a standard size and shape so that the results for different materials can be compared.
Depending on the type of material, an extended yield point (yield-point runout) or a continuous transition from the elastic region to the plastic region (with 0.2% offset yield point) can occur on the curve.
The following two characteristic curves are examples - they can differ from each other considerably depending on the material or its variation. Stress-strain curve - with 0.2% offset yield point -
Stress-strain curve - with extended yield point -
Strain in % Elastic region
Strain in % S421_093
The normal unit from the international measuring system, i.e. pascal (Pa), is used. Due to the very high values, megapascals (MPa) are mainly used: 1MPa = 1,000,000Pa. The measuring unit newton (N) per square millimetre is still also used, however: 1MPa = 1N/mm2.
Analysis of the stress-strain curve A detailed analysis of the stress-strain curve provides a range of information among which the following should be highlighted:
Yield point ReH and ReL At the start of load application, the strain on the sample is elastic, i.e. the sample rod returns to its original length once the load is removed. This elastic behaviour continues until the yield point ReH is reached. Therefore this point can also be called the elastic limit. (This is an example and a simplified approach for this self-study programme. In practice, there are, of course, numerous variants of the curve where, for example, the elastic limit can be just in front of the yield point. These cases will, however, not be examined further in this self-study programme). The elastic limit separates the elastic region from the plastic region. The sample starts to deform plastically once the yield point ReH (elastic limit) has been passed. Depending on the type of material, the yield point can also cover a region (the yield-point runout “X”) with an upper yield point ReH and a lower yield point ReL (see figure S421_008). If there is no extended yield point, the 0.2% offset yield point is set as a substitute yield point. This is the point where the 0.2% remaining strain is found. A line is drawn parallel to the linear rise at a distance of 0.2% strain for this purpose. The point where this line crosses the curve is the offset yield point Rp 0.2 (see figure S421_093).
Ultimate strength or tensile strength Rm The stress reaches maximum here. The stress Rm is the highest load that a cross-section can withstand. From this point on, the sample starts to neck, i.e. the cross-section area becomes smaller. Since the stress is calculated as a force in relation to the cross-section area, the force required for further deformation decreases after point Rm.
Fracture point (Z): The sample fails at this point. This value has no significance for technical practice.
Basics - Materials Basics - Steel Steel is one of the most common materials in vehicle body construction. Steel is an ALLOY of iron and carbon with a maximum carbon proportion of 2.06%. Greater proportions result in castings. Further elements like nickel, manganese, phosphor, silicon, chrome etc. can be alloyed to produce the different steel families. There are a large number of steel types, each of which has a different composition and thus different properties.
Production of steel Iron ore extraction
Foundry ladle Distributing trough
Ore charging Furnace Ingot mould
Billet discharge S421_070
The iron ore found in the ground is smelted in a furnace to form iron (pig iron). Depending on the composition of the iron ore used, the smelted pig iron has its own specific composition. The resulting pig iron is then processed at the steelworks to adjust its chemical composition to previously specified and required values. This can be achieved by removing and adding certain elements. The process is also called alloying.
Different types of steel can be produced by varying the carbon content and other alloying elements. Setting the carbon content up to around 2.06% in particular makes a steel from the iron. The specific properties of the steel can be specially configured depending on the later use of the material.
At the steelworks, the melt is conveyed to the continuous casting plant and processed into a billet. This billet material then forms the basic product for all further processes, for example, rolling, thermal treatment and surface coating, to produce a wide range of SEMI-FINISHED PRODUCTS.
The steel properties are determined by the following main variables: ● ●
the chemical composition of the steel the later treatment of the steel products
Chemical composition Each type of steel has its own crystalline structure in solid state. This structure gives it mechanical properties that can be determined using a metallographic analysis. One very important aspect of steel production is the speed at which the raw materials are heated and cooled in both the manufacturing process and subsequent procedures. If you examine iron in its pure state, you can determine how its crystalline structure and its magnetic properties and its solubility vary as the temperature rises or falls. To give a better understanding of the properties of a type of steel, first the properties of pure iron, then the properties of different iron-carbon ALLOYS and finally the properties of ALLOYS made from iron, carbon and other components will be explained.
Pure iron To provide a basis for all further observations of the steel types, the temperatures at which pure iron changes its crystalline structure, i.e. the arrangement of its ATOMS need to be known. This new arrangement requires a certain amount of time during which the temperature remains constant. The temperatures where the structure changes are called “critical points” (see diagram “Transformation points of pure iron” on the next page). These “critical points” are shown on the diagram as horizontal lines resembling steps.
Basics - Materials
Transformation points of pure iron e
Alpha iron or ferrite Cooling curve
Heating curve S421_009
Heating At temperatures between 0 and 790°C, iron is called “alpha iron” or “ferrite” and has a body-centred cubic crystalline structure consisting of nine iron atoms. Alpha iron is very magnetic and does not dissolve carbon.
Between 1,400 and 1,535°C, it is called “delta iron”. The crystalline structure is body-centred cubic. Since it only occurs at very high temperatures, it is only of little importance in the investigation of thermal treatment types.
If the iron is heated further to 790 to 910°C, it is called “beta iron”. It still has a body-centred cubic crystalline structure that also does not dissolve carbon, but it loses part of its magnetism.
At temperatures above 1,535°C, pure iron is liquid. In comparison with heating, the opposite process occurs during cooling (with minor deviations in the “critical points”).
Between 910 and 1,400°C, it is called “gamma iron”. The cubic structure becomes face-centred at this stage. Gamma iron is not magnetic and dissolves carbon.
At the “critical transformation points”, the absorbed heat is used to change the crystalline structure. Therefore there is no rise in temperature. This means that the iron atoms group themselves in different crystalline structures with different magnetic properties and different carbon solubility depending on the temperature.
Transformation points of iron-carbon alloys Steel crystallises in different microstructures depending on the temperature and carbon proportion. Steel is an iron-carbon alloy with a maximum carbon proportion of 2.06%.
Temperature in °C
Melt Austenite + melt Austenite Austenite + cementite
The illustration shows only the area of the iron-carbon diagram that is relevant to steels. The complete version of the diagram reaches to over 6% carbon.
Ferrite + austenite Ferrite
Pearlite + ferrite
Pearlite + cementite
S421_010 Carbon in %
Interpretation of “iron-carbon diagram” The lines on the diagram show the “critical points”, at which the steel changes its crystalline structure. Depending on the carbon proportion, the temperature at which the structural change occurs varies. The areas bordering on the “critical points” show the crystalline structure that the steel adopts in each case. At high temperatures, the steel is molten and all of its components are dissolved - like salt in water. As the steel cools, parts of the iron and the carbon solidify. The so-called “austenite crystals” form (the solidification temperature varies depending on the carbon proportion). If the temperature decreases further, the ALLOY solidifies completely to become austenite. Under approximately 723°C, austenite can form two different structures depending on the carbon proportion in the ALLOY: ●
If the carbon proportion is below 0.8%, austenite becomes pearlite and ferrite, which are distributed within the steel in crystal form. If the carbon proportion is 0.8%, the steel will only contain combined pearlite crystals. If the carbon proportion is greater than 0.8%, austenite becomes pearlite and cementite.
Basics - Materials Structure types The table below explains the most important structural and mechanical properties of the compositions listed in the iron-carbon diagram (only the area of the diagram relevant to steel). (The listed compositions also occur above this area i.e. with > 2.06% carbon.)
Type of microstructure
Ferrite consists of alpha-iron crystals, which form a body-centred cubic crystal lattice. Carbon is deposited between the iron atoms (interstitial SOLID SOLUTION). Ferrite is the softest component of steel. In terms of mechanical properties, ferrite is characterised by an ultimate strength of 28MPa and a strain of 35 to 40%.
Pure carbon atoms can be connected to each other in two ways. Graphite or diamond results depending on the type of bonding. Of course, for steels, only carbon in the form of graphite is important. Its bonds are weak and therefore easily broken. Carbon is either incorporated atomically in the lattice (interstitial SOLID SOLUTION) or in the form of bonds - see, for example, cementite.
Cementite is a chemical compound of iron and carbon. In chemistry, it is known as iron carbide (Fe3C). Cementite contains 6.67% carbon and 93.33% iron. Cementite can be deposited in the structure in a different form, in separate formations (e.g. rods or needles) or in groups on the grain boundaries of the crystalline structure. Cementite is the hardest, but also most brittle component of steel with an ultimate strength of 215MPa.
Austenite consists of gamma-iron crystals, which form a face-centred cubic crystal lattice. It contains carbon, which is deposited between the iron atoms like with ferrite (interstitial SOLID SOLUTION). Due to the larger interstices in the face-centred cubic crystal lattice, more carbon can be incorporated compared with ferrite. The carbon proportion varies between 0 and 2.06%. Austenite has an ultimate strength of 88 to 105MPa and a strain of 20 to 23%. It is characterised by a high wear resistance and low HARDNESS and is the substance that occurs most frequently in steels.
Type of microstructure
Pearlite is a mixture of cementite and ferrite layers that results from austenite transformation. The thickness of the layers depends on the cooling speed. The slower the cooling, the thicker the layers. Pearlite has an ultimate strength of 55–70MPa and a strain of 20–28%. The mechanical parameters of pearlite are between those of ferrite and cementite; it is harder and more resistant than ferrite, but softer and easier to shape than cementite.
Martensite is produced by cooling austenite very quickly. During this process, the face-centred cubic lattice of the austenite is transformed into a body-centred cubic lattice. More carbon is dissolved in the face-centred cubic lattice due to there being more space available than in the body-centred cubic lattice. As a result, the carbon cannot find enough space during the structural transformation, distorts the crystal lattice and expands it. Plate-like crystals are formed, which look like needles in the microsection - so-called martensite needles. The compression stress caused by the greater volume of the martensite results in the greater HARDNESS, but also the brittleness of the martensite. As the cooling speed increases, less and less pearlite is formed so that an almost complete transformation into martensite occurs. After cementite, martensite is one of the hardest components of steel. The ultimate strength of martensite is between 170 and 250MPa and the strain is between 0.5 and 2.5%.
Like pearlite, bainite consists of the ferrite and cementite phases, but differs from pearlite in form, size and distribution. Bainite has a structure containing either bundles of ferrite laths with film-like carbide layers between them or ferrite plates with layers of carbide between them. Bainite is formed by accordingly controlled fast cooling of the austenite at temperatures and cooling speeds between those for pearlite and martensite. After cooling the austenite to temperatures above the martensite start temperature, the conversion into bainite occurs in the so-called bainite phase at a now constantly maintained temperature (isothermal). The cooling speed is controlled so that no pearlite is formed. The ultimate strength ranges between 15 and 220MPa and the strain is 1.5 – 2%.
Basics - Materials In the following section, two examples of structural changes, which occur in the production of steel with a carbon proportion of 0.15 or 1.20%, are explained by way of illustration.
Steel with 0.15% carbon
Liquid phase Austenite
The starting temperature is over 1,500°C - the steel is liquid. If the temperature falls below 1,400°C, part of the iron and the carbon solidifies and a mixture of a liquid phase and austenite is created. When the temperature drops below 1,300°C, the steel with 0.15% carbon proportion is already completely solid and has become austenite. It remains like this until the temperature falls below 750°C. Between 750 and 723°C, a mixture of austenite and ferrite is formed. Below 723°C, the crystalline structure changes and a mixture of pearlite and ferrite is formed. If, during this phase, the cooling speed changes at any point, differing structure components, like, bainite, martensite etc., can form.
Steel with 1.20% carbon
Liquid phase Austenite
This steel type is also liquid at 1,500°C. Between 1,300 and 1,200°C, a mixture of a liquid phase and austenite occurs. When the temperature drops below 1,200°C, the steel with 1.20% carbon is completely solid and has become austenite. Between 1,000 and 723°C, a mixture of austenite and cementite is formed. At temperatures below 723°C, the crystalline structure is transformed into a stable state and forms a mixture of pearlite and cementite.
Basics - Materials Alloying steel with further components The carbon proportion is responsible for the STRENGTH of the steel. If selected further alloy elements, for example, silicon, phosphor, titanium, niobium or chrome are added, other specific properties can be created as required. The effects of these elements are even noticeable if they are added only in small quantities in relation to the other alloy components. The ALLOYING of an iron-crystalline structure can happen in the following different forms: ●
Substitution: ATOMS of other elements replace iron atoms in the crystal matrix. Gap: Iron atoms are removed from the crystal matrix and the corresponding space remains free. Interstitial: ATOMS from other elements like titanium occupy interstitial* positions between the iron atoms of the crystal matrix. They hinder possible sliding of the atom surfaces against each other and thus increase the strength, for example. Their quantity in the steel alloy is decisive for the later mechanical properties.
Interstitial - located in an intermediate position within a structure
Crystalline structure/crystal matrix
ATOM of base material
The table shows you how the steel properties can be influenced with examples of some further important alloy elements.
Changed properties of the steel
Increases the passivity of the steel towards corrosive influences (it is the main alloying element for increasing the rust- and acid-resistance of steels)
Refines the grain; increases the STRENGTH; improves the temperability; increases HARDNESS, strain and wear resistance; improves weldability and malleability
Increases the STRENGTH and the tenacity; enhances the passivity of the steel towards corrosive influences; improves the temperability, reduces the tempering brittleness in CrNi and Mn steels; favours fine grain formation and improves the weldability.
Increases the STRENGTH and tenacity; contributes to stabilisation of the austenitic lattice structure; improves the formability even at low temperatures
Niobium behaves similar to titanium
Increases the STRENGTH; contributes to an equal balance between press-formability and mechanical STRENGTH
Increases the STRENGTH and the elastic limit; refines the grain
Increases the STRENGTH of austenitic steels; improves the mechanical properties at higher temperatures
Increases the STRENGTH and tenacity; inhibits grain growth and thus contributes to a fine-crystal microstructure; suppresses the precipitation of chrome carbide in chrome alloy steels and thus grain boundary corrosion
Basics - Materials Basics - Treatment of steel There are numerous types of treatment that can be grouped into three large families:
Cold forming Hot forming
Hardening Annealing Normalising Tempering
Case hardening Carbonitriding Nitrating
Mechanical treatment This includes processes in which permanent forming of the metal occurs using mechanical energy. These processes do not have an effect on the crystalline structure, but instead change the elasticity, tenacity, plasticity and HARDNESS.
The most common mechanical processes are:
The steel is formed below its RECRYSTALLISATION temperature. The HARDNESS, the deformation resistance and the elasticity limit of the steel are increased.
The steel is formed above its RECRYSTALLISATION temperature. In this treatment, plastic deformation and the RECRYSTALLISATION of the deformed grains occur simultaneously whereby the temperature has to be maintained long enough so that complete RECRYSTALLISATION occurs. This treatment allows the same forming as in cold forming, but with less force requirement resulting in softer, more malleable steels with a more standardised crystalline structure.
Thermal treatment Thermal treatment includes processes in which the properties of the metals are modified by changing their structure and the structural constitution. The resulting material with these new properties can perform the intended tasks better. The application possibilities and performance are much better here than would be the case in normal conditions. Thermal treatment includes the thermal treatment of steel.
In general, thermal treatment is simply “heating and maintaining” a certain temperature in the steel for a more or less long period of time. It should then be cooled in a suitable way. This results in changes to the microscopic structure of the steels that are responsible for the required adjustment of HARDNESS and STRENGTH . This means that, in thermal treatment, only the thermal energy has an effect. This effect is on the crystalline structure, but not on the chemical composition.
The four most important thermal treatment methods are described in the following section:
The steel is hardened by cooling it quickly to avoid renewed changes to the crystalline structure.
The steel is annealed when it has been subjected to deformations through mechanical influences or other causes. The steel is cooled very slowly in this case.
The steel is normalised to remove tension in the steel. The normal state of the steel concerned is produced. A medium cooling speed is required for this.
The steel is heated (tempered) again after hardening. The stability of the structure is improved in the process. Tempering partly reverses the hardening. However, these effects become greater as the temperature to which the material is heated rises.
Basics - Materials Microstructures Thermal treatment methods allow variations in the structural composition of the steel to be achieved. This is, of course, also dependent on the composition of the steel (proportion of alloying elements). The respective variation is obtained using the proportions of certain structural components that have a basic influence on the STRENGTH/HARDNESS of a steel type.
The steel can be adapted to the application requirements with this kind of treatment. This approach is used with the body. Depending on the requirements for the different body areas, steels with the necessary structural compositions and thus also the necessary strength parameters are used.
The basic structural components with their respective strength areas are shown in the diagram.
Elasticity limit Re of selected structural components Bainite: 15–220MPa
Pearlite: 55–70MPa Martensite: 170–250MPa
Cementite: 215MPa Ferrite: 28MPa
Elasticity limit Re
Thermochemical treatment This includes processes in which chemical components are involved in the steel treatment in addition to thermal energy (heat, maintain temperature, cool). The microstructure and the chemical composition of the steel vary accordingly. The most important thermochemical treatment methods are:
In case hardening, the surface of a steel part is enriched with carbon (carburization) creating the conditions for later hardening. The part is heated and kept at a suitable temperature while simultaneously being in contact with materials that can release carbon. The enrichment with carbon can be achieved, for example, by means of gas carburizing, powder carburizing and carburizing in salt bath. During the subsequent cooling, the layers produced are hardened while the noncarburized material core remains unchanged. The process results in greater tenacity and impact strength.
Carbonitriding is actually an advanced variant of case hardening. In this process, the surface of steel parts is also enriched with nitrogen in addition to carbon. The enrichment is performed in a cyanide salt bath at corresponding temperatures. The material is then cooled in a controlled process. There is little warpage due to the low hardening temperatures and the milder quenchant. In this process, hard outer layers with a low thickness are created in a simple and fast way.
Nitration also forms hard layers on the surface of the steel part by forming nitrides. These layers reach a high level of HARDNESS that is even greater than the HARDNESS of the layers formed in case hardening (see above). This process is based on steel absorbing nitrogen in its microstructure. The process occurs at low temperatures which is why deformation is minimal. There is no quenching and no transformation of the structure.
Basics - Materials Basics - Aluminium Weight is playing an increasingly important role in vehicle design. This results in particular from constantly rising targets for economic and environmentally friendly vehicles.
Full aluminium bodies are not used for Volkswagen vehicles. Aluminium is used for individual selected components, for example: ●
In addition to optimised solutions in body design, lower weight can be achieved by using lighter materials. Aluminium, for example, is being used more and more.
Doors and lids on Phaeton Bonnet on Touareg
Production of aluminium Aluminium is extracted from bauxite in a digestion process using caustic soda (NaOH). This method is called the Bayer process. Bauxite: Bauxite ●
Formed by the weathering of limestone and silicate stone in the appropriate climatic conditions The name comes from its place of discovery, Les Baux (southern France).
Aluminium oxide Silicon oxide
It is difficult to extract the aluminium from the ore as it is in a very stable oxide bond with oxygen. It cannot therefore be extracted from the ore by smelting with the aid of carbon as in iron production.
Aluminium is readily found on Earth, but economic extraction has only been possible for around the past 100 years.
Not until the end of the 19th century was it possible to produce aluminium on a large scale using electrolysis with the dynamo invented by Werner von Siemens.
Primary aluminium pig
On an industrial level, the extraction of aluminium by electrolysis is performed in large iron vats of molten aluminium oxide that are lined with a coating of carbon. The vat serves as the cathode. Carbon blocks submerged in the aluminium oxide are used as anodes.
Molten aluminium oxide
The aluminium is deposited on the floor of the vat since the distance to the floor is shorter than to the side walls. This causes a layer of liquid aluminium to form under the molten aluminium oxide. The aluminium is tapped off every 2–4 days and can be cast in bars.
Carbon block anodes
Alloying aluminium Aluminium alloys are used instead of pure aluminium to guarantee optimum material properties for the respective body components. Aluminium is low STRENGTH in its pure state. The properties of aluminium can be changed by adding other elements, i.e. by ALLOYING . This concerns primarily the STRENGTH and the corrosion resistance. The most frequent alloy components are magnesium and silicon. These ALLOYS then form the basis for extruded profiles, cast nodes and aluminium sheet.
The STRENGTH of aluminium alloys can be increased by forging and curing. One decisive requirement for the usability of aluminium in technical applications is its curing capability. In curing, precipitation of brittle structure components within the alloy structure can be achieved with specific temperature control. This builds up inner resistance to deformation and results in an increase in STRENGTH.
Steels for Body Construction Classification of steels for body construction Due to the large number of possible steel types, it is useful to classify them according to specific features. This allows steels to be classified according to their mechanical values, for example, ultimate strength and yield point. One example is the differentiation of conventional, high-strength, higher-strength and ultra-high-strength steels.
Classification according to strength
Ultimate strength in MPa
Classification according to steel family
Up to approx. 300
Micro-alloyed steel; Isotropic steels
Grain refining and precipitation hardening
Phosphor-alloy steel Interstitial-free (IF) steel
Solid solution hardening
Dual-phase (DP) steel
Transformation induced plasticity (TRIP) steel
Complex-phase (CP) steel
Ultra-high-strength thermoformed steels
It is possible to classify steels according to their mechanical values, but this is imprecise. There is no fixed value for a boundary between the different steels. Normally quite a large bandwidth is involved. There can, for example, be cases where high-strength steels have identical or higher values than higher-strength steels. For this reason, steels are normally and more relevantly also grouped into families according to manufacturing method. Steels from these families will be looked at over the following pages as they are increasingly used in body construction. In particular, the mechanisms for increasing the STRENGTH compared with conventional deep-drawn steels are explained. A balanced ratio between increasing strength and plasticity is decisive here. Basically the STRENGTH of steels can be increased in four ways: ● ● ● ●
solid solution hardening grain refinement and precipitation hardening, bake hardening hardening using hard phases (hard phases = hard structure phases)
Increasing strength of steel Increasing strength - with solid solution hardening Normally, hardening initially calls to mind the thermal treatment of steel for achieving greater HARDNESS. Increasing the STRENGTH and also the HARDNESS can, however, be achieved by ALLOYING with other elements. This method is known as solid solution hardening. The hardening method allows the two steel types higher-strength IF steels (Interstitial Free steels = IF steels) and phosphor-alloy steels to be produced, for example.
ATOM of Fe basic lattice Fe ATOM replaced with substitution (e.g. phosphor)
Alloying material deposited interstitially (IF) (e.g. carbon and nitrogen)
Higher-strength IF steels: These steels have a ferrite matrix without interstitially (interstitial = inside lattice) dissolved alloying proportions. As early as the steel melt, an accordingly lower proportion of carbon and nitrogen is set with specific treatment. Remaining ATOMS from these elements are bound by microalloying titanium and niobium. The steels have good malleability due to the lack of blockages by carbon and nitrogen (interstitial free). Phosphor and manganese are added to the steel to obtain the required STRENGTH. This is then known as higher-strength IF steel. The steels mostly have a minimum ultimate strength between 340 and 460 MPa or a minimum yield point (here the 0.2% offset yield point RP0.2) between 180 and 340 MPa.
Phosphor-alloy steels: These steels also have a ferrite matrix and contain hardening elements from solid solution hardening with phosphor (substitution), which can have a proportion of up to 0.12%. The steels are characterised by their compromise between “mechanical STRENGTH and press formability”, which is why they have a wide range of applications, for example, in structural or reinforcing parts (longitudinal members, crossmembers, pillars etc.), parts that need to be fatigue-resistant or parts that play an important role in crashes. These steels mostly have a minimum ultimate strength between 340 and 480 MPa or a minimum yield point between 220 and 360 MPa.
The steels have a good balance between press formability and mechanical STRENGTH. If repairs are required, the steels weld well in any welding method.
Steels for Body Construction Increasing strength - by means of grain refinement/ precipitation hardening
The STRENGTH of a steel can also be increased by reducing the grain size (grain refinement) and with precipitation hardening. This principle of grain refinement is used, for example, for micro-alloyed steels. Vanadium, niobium and titanium are alloyed in small quantities. This micro-alloying creates a fine dispersion of carbide/nitride precipitation during hotrolling. The grain growth is limited by this and ferrite grains measuring 1,000MPa >800MPa
Steels for Body Construction “DP” (dual-phase) steels DP steels have a high mechanical STRENGTH and good malleability. The ultimate strength Rm is between 500 and 600MPa.
Metal strip Temperature
The STRENGTH is achieved by fast cooling of the hot metal strip - immediately after the rolling process – in the ferrite area. A cooling pause in the ferrite area allows the formation of sufficient ferrite. Then it is cooled more quickly to a low reeling temperature so that the remaining austenite is turned into martensite.
The cooling speed and the steel composition are adjusted to each other so that no pearlite and as little bainite as possible are formed. A mixed structure results with approx. 80–90% ferrite and 10–20% insularly deposited martensite.
“Dual-phase steels” contain approximately 0.12% carbon, 0.5% silicon and 1.46% manganese. * Reel = reeling device for hot metal strip
“TRIP” (TRansformation Induced Plasticity) steels
The STRENGTH is achieved by fast cooling of the hot metal strip - immediately after the rolling process. It is cooled in the ferrite area where ferrite is formed in a cooling pause. The austenite is enriched with carbon during this process. Then the bainite area is cooled and the hot metal strip is reeled up. The enrichment of the austenite with carbon continues. If the martensite starting temperature is below room temperature, the austenite that has not yet been transformed remains as so-called “residual austenite” in the structure. Undesired martensite forming in the bainite is prevented by suitable ALLOYING. The temperature of the reel is decisive for the process.
TRIP steels have a very good ratio of STRENGTH and plasticity; the ultimate strength Rm is between 600 and 800MPa. Ferrite
Bainite Martensite Time S421_029
“TRIP” steels have up to 20% residual austenite in their structure. This residual austenite is not transformed into martensite until the material is shaped later on and is hardened in the process. TRIP steels normally contain about 0.15–0.4% carbon, 1–2% silicon and 0.5–2% manganese.
“CP” (complex-phase) steels
CP steels are characterised by high energy absorption and high deformation resistance. The STRENGTH is achieved by fast cooling of the hot metal strip - immediately after the rolling process. It is cooled quickly to a reeling temperature in the bainite range and then reeled. Only a small amount of ferrite and martensite is formed. Micro-alloying additives like niobium and titanium are used for grain refining. This gives the steel a very finegrained structure.
CP steels mark the transition to the ultra-high-strength steels, which can have an ultimate strength value Rm of over 800MPa.
Martensite Time S421_097
CP steels have a low carbon proportion of less than 0.2%; furthermore they contain alloying elements like manganese, silicon, molybdenum and boron.
“MS” (martensite) steels
The STRENGTH is achieved by cooling the hot metal strip at maximum speed - immediately after the rolling process. In the process, it is cooled to approximately 200°C and the strip is reeled. A predominantly martensitic microstructure is thus produced. Due to the high STRENGTHS over 1,400MPa, thermoforming is necessary for the later shaping of parts made from martensitic steels.
MS steels are among the highest-strength steels. They are characterised by ultimate strength values Rm of around 1,000MPa to over 1,400MPa. Ferrite
Bainite Martensite Time S421_098
As even small ferrite proportions need to be avoided due to the danger of material properties being dispersed, the transformation is controlled as required by alloying Mn, B and Cr. The STRENGTH is controlled via the carbon content.
Steels for Body Construction Body structure Overall, the body structure is the most important and central part of the body.
Taking the latest Golf as an example, we will show the different materials that are used in the body assemblies
Today, modern bodies need to meet extensive and very complex requirements. They are therefore optimised according to the following main points: ● ● ● ● ●
Passive safety Lightweight construction Stability and vibration resistance Pedestrian protection Corrosion protection
In addition to the geometric/constructive design of the SEMI-FINISHED PRODUCTS and profiles, this optimisation is achieved by using tailor-made materials with different strengths for the respective body areas. Steel is used more than any other material. Aluminium and plastics are also used to create lightweight constructions. Sheets with higher STRENGTHS are increasingly being used – the greatest STRENGTH is provided by thermoformed ultra-high-strength sheets. What characterises these sheets? They are steel sheets that are formed in heated state, for example, at temperatures between 900 and 950°C. A defined cooling process produces a microstructure that provides greater STRENGTH and HARDNESS. There are also die-quenched sheets. These allow, for example, very slim and light body parts to be produced without losing strength.
Ultra-high-strength sheets in the assemblies: ● ● ● ●
Inner A-pillar Seat brackets Outer side member Front brackets on front longitudinal members Rear bumper cross member
Legend Steel sheet up to 140MPa High-strength steel sheet from 180 to 240MPa Higher-strength steel sheet from 260 to 320MPa Ultra-high-strength steel sheet from 340 to 700MPa
Thermoformed ultra-high-strength sheets in the assemblies: ● ● ● ● ● ●
Front bumper cross member Cross member in footwell area Inner side members Centre tunnel A-pillar/roof frame area B-pillar
Ultra-high-strength, thermoformed steel sheet over 1,000MPa
The strength figures in MPa refer to Rm = ultimate strength. 1 MPa = 1 newton/mm2
Basics - Process Engineering Manufacture of semi-finished products Constantly greater and also more differentiated constructive requirements are being set for modern bodies. To meet these requirements, the materials/SEMI-FINISHED PRODUCTS are selected and used so they are precisely tailor-made for the load profile. The body calculations and later tests provide load curves within the body that can be predicted increasingly closer to practice thanks to today’s computing possibilities.
Design and calculation
Laboratory and practical tests
The calculations and tests are used as a basis for the configuration of the body structure: ● ● ●
Defining the semi-finished product profile Selecting the semi-finished product material Selection of the respective body parts and their material that will be treated during production (e.g. hot forming in forming die) Selection of the body areas and the respective parts that have cross-section variations within the part (tailored blanks)
Forming process Different processes are used to produce SEMI-FINISHED PRODUCTS. Today’s thin steel sheets are ideal for meeting the requirements of lightweight construction while simultaneously providing high STRENGTH to meet safety requirements. However, they also need accordingly good malleability for shaping. This shows how complex the requirements are!
The main forming methods are: Deep drawing
Basics - Process Engineering Deep drawing In deep drawing, the sheet metal is formed by using the simultaneous effect of pulling and pushing forces. The sheet metal is shaped in one or more operations. Materials with corresponding deformability are used deep-drawn sheet. One special type of deep-drawing is stamping. Embossed structures and shapes, for example, inscriptions, can be added to the surface - this is often performed simultaneously with the deep-drawing process, however.
The cut sheet metal is placed on the drawing die …
Blank Drawing die
Forming force Holder
… and clamped by the holder.
The punch is then pushed downwards and draws the sheet metal over the drawing edge into the opening in the drawing die. The sheet metal is pressed so firmly onto the drawing die by the holder that creases cannot form in the flange area.
Upon completion of the drawing process, the punch releases the workpiece as it moves upwards.
Hydroforming Hydroforming uses pressure to shape metal. In this process, high pressure is used to press a sheet-metal profile against a hollow mould. This method also allows parts with different and complex geometries, e.g. with subsections, to be produced very quickly. Furthermore it allows weld seams to be avoided. The strain hardening that occurs during forming increases the component strength or stiffness.
The sheet-metal profile is placed in the lower half of a two-piece die.
The die is then sealed and filled with a liquid pressure medium.
The liquid pressure medium is then pressurized to approx. 170MPa. The resulting forces press the inserted sheet-metal profile against the die and thus produce the required new form.
Upon completion of the forming process, the mould halves separate and the finished formed part can be removed.
Finished T piece
Basics - Process Engineering Impact extrusion Impact extrusion uses pressure to shape metal. The materials used in this process need to have a high level of malleability.
Starting shape (slug)
In impact extrusion, materials are pressed into solid or hollow parts using a punch and a die. A slug is placed in the forming die as the starting material. When the punch pushes this material together under high pressure, it is forced on the other side into the die opening. Forming hardens the material. Furthermore a corresponding surface quality can be achieved with the die.
Rolling Rolling uses pressure to shape metal. Roller
Profiles, sheets, tubes and wires are fed between rotating rollers and shaped in the process. The material is compressed by the rollers and thus hardened accordingly. Furthermore the desired surface qualities can be produced.
Extrusion uses pressure to shape metal. Billet
In this process, heated materials are pressed through a die and extruded as a billet. Different profiles can be produced depending on the shape of die used.
The material is compressed by the reshaping in the die and thus hardened accordingly. Block
Furthermore the desired surface qualities can be produced.
Basics - Process Engineering Tailored blanks As the term “tailored” indicates, tailored blanks are parts that are made to measure. “Blanks” are the starting material. Tailored blanks were originally developed to produce sheet metal plates with widths that could not be produced with the rolling technology of the time. Today, producers make use of the advantage that tailored blanks allow different steel grades and sheet thicknesses to be joined together in a finished part.
Tailored blanks allow an increasingly better and more precise adjustment of the body structure to the loading of certain body sections. This allows parts with complex shapes and precisely fitting designs to be produced. The individual parts of the tailored blanks are joined together by welding. After welding the blank is then shaped, for example, by deep drawing.
Example - floor pan - front with tailored blanks
Front longitudinal member Increasing sheet thickness
Different welding methods are used to join the individual components of tailored blanks. One method that was frequently used in the past was mash seam welding. Today, this has, however, mostly been replaced by more modern laser welding. Therefore we will not look further into mash seam welding. The seam edges must be prepared well to obtain the necessary seam quality in laser welding.
... joining with laser welding
Laser nozzle Welding rod feed Laser beam
Welding rod S421_095
In addition to laser welding, high-frequency welding is also used for tailored blanks today. ... joining with high-frequency welding In this process, metal sheets are clamped at a defined gap “x” from each other.
Clamping jaws/electrodes Sheet metal
The high-frequency current is conducted directly through the sheets via clamping jaws/electrodes. Electrodynamic effects cause the welding current to be concentrated on the edges of the sheets. Once the necessary temperature has been reached, the current is switched off and the heated joining edges are squeezed together.
S421_069 HF connection
S421_084 Protruding seam
Extremely short welding times can be achieved with high-frequency welding. The requirements for the seam preparation are fewer than in laser welding. Even non-straight seams can be welded easily. One disadvantage of the process is the protruding seam left upon completion of the welding process. The seam needs to be reworked afterwards.
Basics - Process Engineering Joining processes Monocoque bodies need a structure that provides the necessary stability and stiffness - without a supporting frame. The joining methods used to produce the body are very important. Parts are connected to each other in joining.
The following joining methods are used for body construction: Frictional connection: ●
Frictional connections, for example, screw joints, represent only a small proportion of the joining methods in body construction today. The necessary requirements for stability and stiffness of the body cannot be met with screw joints.
Positive-fit connection: ●
Rivet joints are among the positive-fit connections. At least two parts are interlocked and connect the parts. Rivet joints also only meet the requirements for stability and stiffness to a limited extent.
Firmly bonded connection: ● ● ●
Weld joint Solder joint Adhesive joint
The aforementioned requirements can be easily fulfilled with firmly bonded connections. These joining methods produce a material compound since material is mixed in the join gap, e.g. in welding. Parts joined in this way can be considered to be more or less a new part. Material mixing does not occur during soldering and bonding. However, direct contact in the join gap is considerably more intensive so accordingly high STRENGTHS can be achieved.
Screw joint Screw joints have the advantage that repairs and replacement operations are easy and cheap to perform.
Screws for front cross member on Passat 2006 (example)
However, the disadvantage is that the body stiffness normally required for today’s monocoque bodies is very difficult to attain. In many cases, the advantages are minor compared with the advantages of a firmly bonded connection. A very stiff body is important with regard to crash safety in particular and also in general driving. S421_040
Screw joints reach their limits here. For this reason, screw joints are used, above all, in places where the load bearing capacity of the body structure is not an issue.
Front cross member (Passat 2006)
Furthermore attachments are mounted with screws to a great extent. Where are screw joints used, for example? ● ●
Screws for front left wing on Golf 2004 (example)
Fastening wings to the body structure Securing the front cross member to the longitudinal members
Front left wing (Golf 2004)
Basics - Process Engineering Rivet joint Punch riveting Punch riveting involves a semi-hollow rivet being pressed through the first layer of sheet metal. The second layer of sheet metal is only deformed by the rivet and is not penetrated. The foot of the semihollow rivet spreads and forms a closing head that gives the rivet joint the necessary hold.
Riveting tool (upper part) Semi-hollow rivet 1st and 2nd sheet layers Riveting tool (lower part) S421_050
Advantages: ● ● ●
No pre-drilling of sheets Second layer of sheet metal is not cut Greater STRENGTH and lower energy requirement than with resistance spot welding
Steel is used as a material for punch riveting. If the rivets are used for aluminium sheets, they need to have a zinc/nickel coating to avoid galvanic corrosion.
Clinching Clinching is used to connect non-load bearing simple components as the connection point only has a low STRENGTH. Rivets are not required here. The punch presses the two sheets into a die at the joining point. By sinking and clinching the upper sheet into the lower sheet, a frictional and positive-fit connection is formed.
Punch Upper and lower sheet Die S421_053
Advantages: ● ●
Fast and clean joining technique Low cost
If the sheets are made from different materials, an electrochemical insulation coating is required to prevent galvanic corrosion.
Blind riveting Blind riveting can be used whenever the riveting point can only be accessed from one side.
The illustrations show an example of blind riveting using pop rivets.
Rivet gun Mandrel
Pop rivets are hollow rivets with a mandrel. The pop rivet is inserted into the aligned holes of the parts being connected with a rivet gun.
Parts being connected
The gun now pulls the mandrel back. This causes the mandrel head to expand the protruding rivet body and form the closing head. The mandrel then snaps at its break point. S421_057
The rivet gun is removed with the broken-off mandrel. The rivet joint is complete.
Basics - Process Engineering Welding Today laser welding and electric resistance welding are used for a wide range of welding applications. Therefore both methods will be looked at as examples of welding. In addition to laser welding, plasma welding - a further development of TIG welding (TIG = tungsten inert gas) - is also used. This method is currently not very widespread in body construction and will therefore not be looked at here.
Laser welding In laser welding, the heat to melt the materials is produced by a laser beam. Laser welding was first used to produce tailored blanks for body construction. It is finding increasing use in the assembly of vehicles thanks to many advantages:
Laser welding allows an “almost seamless” connection of parts - this is particularly advantageous for connecting higher-strength sheets. The structural behaviour of the material is also largely retained in the area of the seam. Complicated seams, for example, single-sided welds, are possible. In addition to butt welds, the use of an additional rod also allows other types of seam, for example, hollow welds.
At high working speeds, a very good surface quality is obtained.
The surface of a laser weld seam is already so good that reworking, for example, for a good paint finish, only requires a minimum amount of time.
Examples of laser weld seams on the Passat 2006: ● ● ● ● ● ●
in the area of the door apertures on the front and rear roof member on the lateral windscreen frame in the area of the front wheel housing in the area of the rear window frame on the rear cross panel
Welding rod feed Laser beam
In laser welding, the materials to be joined and the welding rod are liquefied by the high energy of the laser beam. Sheet metal S421_059
Electric resistance welding This method allows electrically conductive materials to be welded. An electrical current flowing through the welding joint melts the material and the parts are welded together - without additional material. Normally low voltages and high currents are used so that the welding effect is possible, but there is also no danger. This welding principle is applied in different ways, for example: ● ●
Resistance spot welding Resistance butt welding
Resistance spot welding: Electrode
Resistance spot welding continues to be very important in body construction. Today, new modern possibilities in control and regulation allow resistance spot welding to be also performed on higher-strength and coated sheet metals. In modern body construction, adhesive is also added to the joining level to improve the structural behaviour and stiffness of the join and increase the vibration resistance. The adhesive layer also prevents penetration of substances, for example, water or other liquids and thus also helps prevent crevice corrosion. One variant of resistance spot welding is resistance roller spot welding that uses rollers as electrodes. The parts being joined run between the two electrodes and a weld seam is produced.
Sheet metal S421_067 Electrode
Resistance butt welding Resistance butt welding is only used on joints that do not carry any loads. Two parts are pressed together and connected to a current. The material melts and is welded at the pressure point. In body construction, this is used, for example, to weld bolts to sheet metal parts.
Pin Sheet metal
Basics - Process Engineering Soldering In contrast to welding, the actual parts being joined are not melted at the joint in soldering. An additional material made from bronze, the solder, is used. The melted solder fills the space at the joint and connects the parts being joined with a high STRENGTH . Due to the low temperatures used for soldering, the zinc coating on galvanised sheet metal, for example, is affected to a lesser extent and substantial hardening is avoided in the join area. Join gaps can be bridged better by the solder. The lower process temperatures allow less heat distortion. The main soldering methods are explained briefly below.
Solder (wire) Wire feed Inert gas nozzle
Clamping sleeve Soldering seam
Tungsten electrode Inert gas nozzle Sheet metal
Wire feed Soldering seam Arc
Solder (wire) S421_122
The solder is melted by the arc between the solder and the part being soldered under the inert gas.
The solder is melted by the arc between a tungsten electrode and the part being soldered under the inert gas.
Plasma soldering Laser nozzle
Laser beam Plasma nozzle
Tungsten electrode Inert gas nozzle
Solder (wire) Sheet metal Wire feed
Soldering seam Wire nozzle
Compared with TIG soldering, the arc is additionally constricted by a plasma nozzle in plasma soldering. This allows a higher energy density and narrower seams. Also higher soldering speeds are possible.
Soldering seam Wire nozzle
In LASER soldering, the soldering heat is produced by a laser beam.
Bonding Bonding is a method for the permanent connection of components using an adhesive. Depending on the type of adhesive, the hardening process can be supported by heating the bond slightly. Thanks to the continued development of new, more efficient adhesives that are tailored to the applications, adhesives and bonding processes are becoming increasingly important in body construction. Bonded joints can even be STRONGER than welding points, for example.
Bonding is not just used to join parts together, however. In body construction, in particular, the method is used for a range of other tasks, for example: ●
● ● ● ● ●
Sealing the joint area against penetrating moisture or corrosive substances Joining different materials, for example, steel sheet with plastics Noise and vibration insulation Gas and liquid sealing Increasing component stiffness Avoiding crevice and galvanic corrosion Low-warpage joins by avoiding temperature loading Cross-area application of force
S421_043 Body part
Appropriate preparations are necessary for proper bonding, for example: ● ●
Surfaces should be clean and free of grease A primer should be applied (bonding agent)
Different adhesives are used depending on the application. They differ … … according to composition
… according to processing temperature
Cold adhesives (room temperature)
Hot adhesives (120–250°C)
Basics - Process Engineering Coating processes The aim of the different surface coatings is to protect the steel in the body against possible oxidation (CORROSION) due to the effect of air and weather. Different coatings are used, but coatings based on zinc are most common. In production today, the body is not completely galvanised by immersion, for example; the body components or their initial SEMI-FINISHED PRODUCTS will in fact be coated before further processing. Zinc is a material that, compared with steel, tends to oxidise more greatly. This results from its position within the electrochemical series - according to the table, zinc is less precious than steel.
The zinc coating covers the steel surface and thus protects it against CORROSION. Optimum protection is provided as long as this coating system is not damaged - for example, by mechanical intrusion. If, however, there is an intrusion which damages the zinc coating and reveals the surface of the steel, contact with water, for example, can lead to premature disintegration of the zinc coating due to the potential difference between the two different materials. The surface of the steel is then exposed and CORROSION starts on the respective steel surface areas. Optimum protection is achieved if the zinc coating is combined with a coat of paint. This is known as a “duplex system”.
The following are normal zinc coating methods for bodies:
Hot dip galvanising for all parts that are not visible from the outside
“Galvanealed” and zinc electroplating for all outer skin panels
Zink coating approx. 10 micrometres
Zink coating approx. 8 micrometres
Hot dip galvanising
Hot dip galvanising cannot be used for outer body panels due to the high process temperatures and the risk of the metal becoming warped.
Production line for deep drawing Zinc bath
Coiled galvanised metal strip
Heating for zinc bath
Hot dip galvanising is performed after rolling and before deep drawing of the sheet metal. After rolling, the sheet metal is immersed in a 450°C liquid zinc bath causing a coating of zinc to be formed. The first coatings of zinc consist of an iron/zinc compound and are followed by a coating of pure zinc. Hot dip galvanising is one of the most effective corrosion protection methods.
Hot dip galvanising is not normally used on visible parts as it leaves a rough surface with markings on the sheet metal. Visible parts would need to be further processed.
Basics - Process Engineering “Galvanealed” method Galvanised metal strip coiled
Production line for deep drawing
Heating for zinc bath
The coating formed in “galvanealing” is added after rolling and before deep drawing of the sheet metal.
Galvanealing provides greater corrosion resistance compared with hot dip galvanising
The “galvanealed” method is a variant of hot dip galvanising. In contrast to hot dip galvanising, the steel is treated thermally (annealed) at 430°C for an additional 30 seconds after the bath.
This method has the following purpose among others: ● ● ●
In this thermal treatment, the iron present in the steel is diffused into the zinc coating. An ALLOY of zinc and iron is formed. The zinc coating contains around 10% iron and is known as a galvanealed coating.
Optimisation of coating weldability Good surface quality without irregularities Good basis for subsequent coatings.
Zinc electroplating Zinc electroplating can be used for outer body panels due to the low warpage.
Cathode (current transfer rollers)
Production line for deep drawing
Galvanised metal strip coiled
Electrolyte liquid Anode
Zinc electroplating is performed after rolling and before deep drawing of the sheet metal. This method is based on an electrochemical process. The metal strip is guided over so-called current transfer rollers, which act as the negative pole (cathode). An electrical field between the metal strip (which now also acts as the cathode) and the anodes acting as the positive pole causes zinc released from the electrolyte liquid to be deposited on the sheet.
This creates a very fine, uniform zinc coating with a thickness of about 8 micrometres. Subsequent processes, like stamping, welding and painting, can then be carried out without losing the corrosion protection. Due to the good final quality, this technique is used for visible parts of the body. The final appearance of the zinc electroplating depends on the coating thickness and the surface quality of the steel.
Corrosion Protection Pre-treatment If the body is to receive a coat of paint, the material must be prepared well. Phosphating is mainly used in body construction for this purpose. Aims of pre-treatment: ● ●
Corrosion protection Creation of a good primed surface
S421_096 Phosphate Body
Phosphating Phosphating is chemical/electrochemical process in which thin fine crystalline water-insoluble phosphates are deposited on the surface of the metal by dipping it into phosphoric acid solutions (iron, zinc or manganese ions and phosphoric acid).
These phosphates are produced in a chemical reaction with the base metal and thus form a layer that is securely anchored to the base metal. Depending on the reacting base metal (this can also be the coating material), a layer of, for example, iron, nickel, manganese or zinc phosphate is formed.
S421_036 Phosphating bath
The coating has numerous hollow spaces and capillaries, which are linked to optimum absorption. This allows good penetration of corrosion protection agents like waxes, oils, colour pigments and paints. Phosphated surfaces thus ensure a good primed surface for paint and lacquer coatings.
Seam sealing Effective seam sealing is equally important for permanent corrosion protection. It is often presumed that, in particular, missed spots in the body cavity sealing are the starting points for CORROSION - today the process of body cavity sealing has been perfected so that hardly any problems can occur in this area. The situation with seam sealing is more critical, however.
At weld seams with overlaps, for example, on ● ● ● ● ● ● ● ● ●
Weld seam with seam sealing
front and rear skirts rear valance engine compartment luggage compartment floor passenger compartment floor side panel wheel housing vehicle underbody wings etc.
the seams require sealing afterwards with suitable sealing materials so that it is impossible for water to get into the spaces between two joined components. Even if, for example, the gaps of weld seams (spot welding) are filled with adhesive, the seams must be sealed. Seam sealing also protects the edges of the sheets. Sealing seams is important because it is virtually impossible for any moisture that penetrates the seams to dry. CORROSION can start in seams considerably faster compared with open surfaces.
S421_038 Seam sealing
Welding spots (spot welding) Adhesive
Corrosion Protection Stone chip protection Stone chip protection is one important and, in practice, also very effective measure against CORROSION. The complete body cannot be treated in this way. Instead coats are applied to the areas of the body that are at risk. This can be done in the following way:
Applying a protective sealant after priming (dip painting) and before applying the paint – e.g. at front end of body. Clear coa t Base coa t Filler coa t Protective sealant Dip pain ting Phospha te Body ma terial
Applying protective sealant after painting (clear coat) to non-visible areas, e.g. to the vehicle floor and the wheel housings, or also applying a special protective film.
Protective sealant/fi lm Clear coa t Base coa t Filler coa t Dip pain ting Phosphate Body ma terial
Stone chip protection is normally a tougher, elastic coating. The elastic properties combined with a greater thickness also have an anti-drum effect. Stone chip protection can also be achieved by using special materials for body parts, for example, by using special plastics instead of painted metal parts.
Protection against galvanic corrosion If other metals, for example, aluminium, are used in addition to steel in body construction, particular attention should be paid to the prevention of galvanic corrosion. This basically also applies to iron/steel. However, due to its particularly low electrical potential value in the electrochemical series, aluminium is considerably more prone to galvanic corrosion. Therefore galvanic corrosion will be explained using aluminium as an example.
Galvanic corrosion All metals have a specific ELECTROCHEMICAL POTENTIAL, which differs from the potential of other metals. If an electrolyte (acidic, alkaline or saliferous liquid) is added to two or more materials that are in contact with each other, voltage equalisation can occur between the potential partners. An electric current flows. The metal with the greater negative voltage value always corrodes first.
The electrochemical series of metals is also used to illustrate the potential differences. Figure S421_046 shows an example of a test set-up to illustrate CORROSION.
Legend for electrochemical series (selection from electrochemical series)
Pb Sn Fe Cr Zn Al
– – – – – –
lead tin iron chrome zinc aluminium
(–0.13 V*) (–0.14 V*) (–0.44 V*) (–0,56 V*) (–0.76 V*) (–1.67 V*)
compared with a standard hydrogen electrode at 25°C Accordingly the potential differences between aluminium and the metals (zinc, chrome, iron, tin and lead) shown in the figure (S421_046) can be calculated from the difference between two metals that are in contact with each other.
Protection against galvanic corrosion Therefore direct contact between components made from different metals should be avoided to prevent galvanic corrosion.
The joint must be designed so that an insulating layer is included between the two different metals.
Variants of an insulating layer can be: ●
Adhesive layer – The adhesive for bonding is used at the same time for insulation
Surface coating of one part – e.g. a bolt for fastening body parts made from aluminium – the coating acts as an insulating layer.
Painting After treatment of the SEMI-FINISHED PRODUCTS or also the complete body, the corrosion protection is concluded with paint. Painting involves the following main steps: ●
Before painting, the body is cleaned and degreased so that no binding faults occur during the painting process. Phosphating then follows to create a good primed surface and meet the requirements for optimum corrosion protection.
● ● ●
Next a cataphoretic dip primer coat is applied. Then the filler coat is applied. After a rinsing process, the top coat consisting of a base coat and a clear coat is applied.
Clear co at Base coa t Filler coa t Stone chip
protectio n/underb ody seala Catapho retic dip nt* primer co at Phosphate Body ma terial
After the cataphoretic dip primer coat, the underbody sealant and the sealant for cosmetic sealing are sprayed onto the appropriate body areas as required. A highly viscous elastic paint is applied to the areas prone to stone chips (see also page 62).
Please refer to SSP 214 “Painting the Vehicle - Pre-Treatment” and SSP 215 “Painting the Vehicle - The Topcoat” for further details on painting. You will also find further information in ELSA (electronic service information system) in “Paint Workshop Manual” (ELSA further above “Internet” button).
Repair Basics The damage needs to be assessed before any repair work is started. Assessment criteria: ● ● ●
In which direction did deformation take place? Are neighbouring, concealed parts of the body also damaged? Has the structure of the body been deformed?
If the body is so badly damaged (deformed) that its structure is also affected, it must be aligned or rectified with the aid of an alignment jig and alignment units.
Alignment unit (example)
Alignment beam Alignment jig (example) Hydraulic cylinder
S421_113 Hydraulic connection
Repair methods Rectification Rectification is the most frequently used repair method for vehicle bodies. Rectification can be done in different ways. Some selected methods are presented briefly below as examples.
Three-point pull directed upwards …
A pull chain is tensioned by a hydraulic cylinder. One end of the chain is secured to the body part being aligned (in this example using additional loop) and the other end to the alignment unit. Hydraulic connection
When the hydraulic cylinder is actuated and extended upwards, the chain is tensioned and pulls the deformed body part upwards.
Loop Longitudinal member Alignment jig Hydraulic cylinder
Directed downwards with loose guide pulley …
One end of the pull chain is placed around a body part, e.g. a longitudinal member, and re-attached to the chain using a chain hook.
Toothed rack on alignment unit
Pull chain Chain hook
The other end of the chain is attached to the toothed rack on the alignment unit.
The pull chain passes through a loose guide pulley with roller and fastening hook. This hook is connected to another chain, which is secured to the lower part of the alignment unit, for example. Hydraulic cylinder
If the pull chain is now tensioned by moving the toothed rack with the hydraulic cylinder, the longitudinal member will be pulled downwards.
Alignment jig Roller holder with hook
Lower part of alignment unit
Repair Direct pressure on chain to pull assemblies downwards A pull chain is laid around the body part being aligned, e.g. the longitudinal member and a suitable frame part on the alignment jig and attached to itself again using a chain hook. This chain loop is tensioned by a hydraulic cylinder.
Pull chain (chain loop)
The hydraulic cylinder attached to the chain loop is actuated. It pushes the chain loop apart and the longitudinal member is pulled downwards.
Hydraulic connection S421_104
Pull chain (chain loop)
Direct application of force to the body with a pressure cylinder to push assemblies upwards This method of alignment uses the telescopic function of the alignment bracket. To start with, the body part being aligned is raised with a hydraulically operated pressure cylinder by applying a force directly.
Telescopic alignment bracket
This process is continued until the telescopic alignment bracket fits under the body and can be locked with a bolt that fits into one of the locking holes.
Telescopic alignment bracket
S421_107 Pressure cylinder
Repair Dent removal with hammer and dolly Dent
If a metal panel becomes dented, the material at the transition points to the normal shape is stretched on the outside while the material is amassed on the inside in a compression. If you hammer back a dent at the centre, the material in the compressed areas will immediately pop up. This means that new stretched and compressed areas will form upon each strike of the hammer.
Outside of dent
As more of these areas are formed, the harder it will become to smoothen out the surface. During dent removal, you should therefore make sure that existing stretched and compressed areas are reduced and no new ones are created. Consequently the dent removal work should normally always be performed from the outside to the centre of the dent. Frequently the metal around the indentation rebounds so greatly that the hammer strike hardly has any effect. “The hammer’s not working!”
S421_115 Centre of dent Working direction for dent removal
It is only when a suitable dolly is held against the back of the metal that measured and effective force can be applied.
There is always a compressed area opposite a stretched area.
S421_116 Stretched area Compressed area
Thermal dent removal method The thermal dent removal method is ideal for dents with a maximum diameter of 10cm and a depth of 1–2mm.
Initial condition of a panel section with a dent
The following principle is used: Metal expands when heated and contracts upon cooling.
If a dent is heated in a spiral starting at the edge towards the centre, the heat will be concentrated in the centre of the dent. This also causes the surrounding body surface to rise slightly
Heating with burner …
Working direction for heating
Now a special body file, which has a convex blade, is used to file over the centre of the dent. The file rests on the edge of the dent and draws off the most heat there. As a result, the deeper material contracts towards the edges and raises the centre of the dent. The file heats up very quickly during the process and needs to be exchanged for a cold file after several back and forth movements.
Heat withdrawal using a file …
Withdrawal of heat
Working direction of file Damaged area after repair …
Important: The file is used for faster heat dissipation, not for removing material!
S421_120 Damaged area
Repair Drawing in an „oil can“ dent with the carbon electrode Carbon electrode
The indented metal surface is heated at certain points with a carbon electrode until it is cherry red. The heating points should follow a spiral from the outside to the inside like when working with a welding torch. If the areas to be drawn in are larger, each point must be cooled immediately after heating (with a wet sponge).
S421_121 Oil can
Smaller areas are heated in a spiral in a single operation so that they cool down again in a spiral shape. Quenching with water also has a drawing-in effect in this case. This drawing-in effect means that something is “pulled in”. In this procedure, it means that the stretched material in the dent area is pulled back to its original smaller dimensions - i.e. “drawn in”. The material can, however, not be compressed as much simply by heating and cooling as with additional direct beating.
Cutting Cutting out damaged parts The job of cutting out damaged parts can only begin once the body has been aligned sufficiently for the alignment brackets to fit the mounting points on the body. One exception to this rule is, for example, the thermoformed B-pillar and the neighbouring body area towards the A-pillar on the Golf from model year 2004. It is virtually impossible to rectify these parts due to the high STRENGTH.
B-pillar (Golf model year 2004)
Hand tools (e.g. hammers and panel cutters), electrical equipment (e.g. one-hand angle grinders) and pneumatic equipment (e.g. body saws and spot weld removers) can be used to cut out panel sections.
Spot weld remover
Glossary Alloy An alloy is a solid solution with metallic properties. The term alloy originates from the Latin word ligare/ later legare, which means bind, tie or combine. Alloying is very important in engineering as adding certain alloying elements to metals, in particular, steel, allows specific material properties to be obtained.
Atom An atom is the smallest chemical particle of an element that cannot be split. It consists of the positively charged atomic nucleus and negatively charges electrons. The atomic nucleus contains positively charged subatomic particles, called protons, and electrically neutral particles, called neutrons. The protons are responsible for the positive charging of the atomic nucleus.
Corrosion In engineering, corrosion refers to the reaction of a metallic material with the surrounding media that causes a measurable change in the material and, at the same time, impairs the function of the component (the term corrosion is also used in other fields, for example, medicine …)
Electrochemical potential First of all, the term potential as used in this context should be explained. When we generally talk about a potential, we mean a certain level in relation to a starting or comparison level. In electrochemistry, the term electrochemical potential is used, for example. This term means that all metals have a specific electrochemical potential that differs from the potential of another metal. The potential values of the respective metals, which can be found in the electrochemical series, are calculated using a standard hydrogen electrode at 25°C.
Electron Electrons are negatively charged subatomic particles. A single electron has the smallest negative charge unit - the elementary charge. Depending on the type of element, an atom can contain one or more electrons. This depends on the number of positively charged protons in the atomic nucleus. A balance of opposite charges, i.e. a balance between the positive and negative subatomic particles, is always sought within an atom.
Hardness Hardness is a material parameter that describes the mechanical resistance of a material against a mechanical influence. Hardness is only related to the strength of a material to a limited extent. A high level of hardness is, however, mostly linked to a high level of brittleness (i.e. risk of fracture …). Therefore a good ratio of hardness and strength must be ensured so that the material can fulfil its task. Hardness is also important when looking at the individual structural components of steels (e.g. hard phases). Corresponding solid solutions with specially created hard components also contribute to increasing the strength of a steel.
Laser The word laser is made up from the first letters from “Light Amplification by Stimulated Emission of Radiation”. In a laser, a medium, for example, a helium/neon gas mixture is raised to a higher energy state by “exciting” its electrons. This energy is then emitted as an electromagnetic wave (e.g. as red light) in a highly bundled form, the so-called laser beam.
Metal ion Metal atoms have electrons that are bound to the atomic nucleus and one or more “free” electrons on the outer electron shell. The atomic nucleus including the bound electrons is also known as the metal ion. Without the aforementioned “free” electrons, it has a positive charge. The electrical force of attraction between the negatively charged free electrons and the positively charged metal ions are responsible for the firm cohesion and thus the strength of the metallic material. This kind of bond is also called a metallic bond as it is a characteristic of all metals.
Recrystallisation Recrystallisation is a process by which the crystalline structure of a metal, which has been altered by cold forming, for example, is reformed and the previous change in properties is reversed.
Semi-finished product As the name says, these are parts that do not represent the final state of a product. The semifinished product is prepared in terms of geometry, treatment and, if necessary, coating so that as little reworking as possible is required during further processing or fitting in the finished product.
Solid solution A solid solution is a mixture of two crystalline solids from at least two different chemical elements. The foreign atoms or ions are randomly distributed. They can occupy interstitial sites (interstitial solid solution) or replace atoms belonging to the other element (substitutional solid solution). The foreign atoms are dissolved in a crystal hence the term solid solution.
Strength Strength is a material parameter that describes the mechanical resistance of a material against plastic deformation or fracture. Tensile, compressive, bending, buckling and shear strength can be distinguished depending on the type of load. Normally the ultimate strength is calculated for metallic materials used in vehicle construction and is employed for the categorisation in different strength classes. However, the yield point can also serve as a basis for certain other steel applications, for example, construction steel. The ultimate strength is defined as the greatest tension that occurs in a material. The tension values are calculated in tensile testing using a sample rod.
© VOLKSWAGEN AG, Wolfsburg All rights and rights to make technical alterations reserved. 000.2812.15.20 Technical status 10.2009 Volkswagen AG After Sales Qualification Service Training VSQ-1 Brieffach 1995 D-38436 Wolfsburg
❀ This paper was manufactured from pulp that was bleached without the use of chlorine.